text: The process of pit nucleation is initiated by the depassivation of the protective oxide layer isolating the metal substrate from the aggressive solution. The depassivation of the protective oxide layer is the less properly understood step in pitting corrosion and its very local and random appearance probably its most enigmatic characteristic. Mechanical or physical damages may locally disrupt the protective layer. Crystalline defects, or impurity inclusions, pre-existing in the base metal material can also serve as nucleation points (especially metal sulfide inclusions). The chemical conditions prevailing in the solution and the nature of the metal, or the alloy composition, are also important factors to take into consideration. Several theories have been elaborated to explain the depassivation process. Anions with weak or strong ligand properties such as chloride () and thiosulfate  () respectively can complex the metallic cations (Me) present in the protective oxide layer and so contribute to its local dissolution. Chloride anions could also compete with hydroxide ions () for the sorption onto the oxide layer and start to diffuse into the porosity or the crystal lattice of the oxide layer. Finally, according to the point-defect model elaborated by Digby Macdonald, the migration of crystal defects inside the oxide layer could explain its random localized disappearance. The main interest of the point-defect model is to explain the stochastic character of the pitting corrosion process.